#------------------------------------------------------------------------------
#$Date: 2022-10-06 01:39:57 +0300 (Thu, 06 Oct 2022) $
#$Revision: 278372 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/71/14/7711438.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7711438
loop_
_publ_author_name
'Ablott, Timothy A.'
'Lu, Kimbal T.'
'Aughterson, Robert D.'
'Zhang, Yingjie'
_publ_section_title
;
 Uranium oxide hydrate frameworks with Er(iii) or Y(iii) ions: revealing
 structural insights leading to the low symmetry
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D2DT02763A
_journal_year                    2022
_chemical_formula_moiety         'O22.5 U5.5 Y'
_chemical_formula_sum            'O22.5 U5.5 Y'
_chemical_formula_weight         1758.08
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_audit_creation_date             2022-07-30
_audit_creation_method
;
Olex2 1.5
(compiled 2021.12.09 svn.r5202d8cf for OlexSys, GUI svn.r6439)
;
_audit_update_record
;
2022-08-07 deposited with the CCDC.	2022-09-29 downloaded from the CCDC.
;
_cell_angle_alpha                111.13(3)
_cell_angle_beta                 103.02(3)
_cell_angle_gamma                106.40(3)
_cell_formula_units_Z            2
_cell_length_a                   8.0890(16)
_cell_length_b                   11.408(2)
_cell_length_c                   11.517(2)
_cell_measurement_reflns_used    16000
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      24.999
_cell_measurement_theta_min      2.037
_cell_volume                     885.2(5)
_computing_cell_refinement       'BlueIce (McPhillips, et al., 2002)'
_computing_data_collection       'XDS (Kabsch, 1993)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.919
_diffrn_measured_fraction_theta_max 0.919
_diffrn_measurement_device_type  'Eiger Detector'
_diffrn_measurement_method       'π  scans'
_diffrn_radiation_type
'silicon double crystal monochromated synchrotron'
_diffrn_radiation_wavelength     0.71095
_diffrn_reflns_av_R_equivalents  0.0543
_diffrn_reflns_av_unetI/netI     0.0541
_diffrn_reflns_Laue_measured_fraction_full 0.919
_diffrn_reflns_Laue_measured_fraction_max 0.919
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            8943
_diffrn_reflns_point_group_measured_fraction_full 0.919
_diffrn_reflns_point_group_measured_fraction_max 0.919
_diffrn_reflns_theta_full        24.999
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_min         2.037
_diffrn_source                   'Australian Synchrotron MX2'
_exptl_absorpt_coefficient_mu    53.474
_exptl_absorpt_correction_T_max  0.4343
_exptl_absorpt_correction_T_min  0.2622
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.1768 before and 0.0850 after correction.
The Ratio of minimum to maximum transmission is 0.6037.
The λ/2 correction factor is 0.0015.
;
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    6.596
_exptl_crystal_description       plate
_exptl_crystal_F_000             1450
_exptl_crystal_size_max          0.015
_exptl_crystal_size_mid          0.010
_exptl_crystal_size_min          0.005
_refine_diff_density_max         3.905
_refine_diff_density_min         -3.693
_refine_diff_density_rms         0.626
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.123
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     136
_refine_ls_number_reflns         2866
_refine_ls_number_restraints     397
_refine_ls_restrained_S_all      1.049
_refine_ls_R_factor_all          0.0480
_refine_ls_R_factor_gt           0.0468
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0788P)²+41.0674P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1402
_refine_ls_wR_factor_ref         0.1422
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2723
_reflns_number_total             2866
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d2dt02763a2.cif
_cod_data_source_block           p-1
_cod_original_cell_volume        885.2(4)
_cod_original_formula_sum        'O22.50 U5.50 Y'
_cod_database_code               7711438
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(O1) = Uanis(O2) = Uanis(O3) = Uanis(O4) = Uanis(O5) = Uanis(O6) =
Uanis(O7) = Uanis(O8) = Uanis(O9) = Uanis(O10) = Uanis(O11) = Uanis(O12) =
Uanis(O13) = Uanis(O14) = Uanis(O15) = Uanis(O16) = Uanis(O17) = Uanis(O18) =
Uanis(O19) = Uanis(O20) = Uanis(O21) = Uanis(O22) = Uanis(O23) = Uanis(O17)
2. Rigid body (RIGU) restrains
 All non-hydrogen atoms
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
3. Others
 Fixed Sof: O17(0.5)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.21520(9) 0.66586(7) 0.83768(6) 0.0141(2) Uani 1 1 d . . . . .
U2 U 0.53313(9) 0.48828(7) 0.67249(7) 0.0152(2) Uani 1 1 d . . . . .
U3 U 0.80372(9) 0.35471(7) 0.48692(7) 0.0123(2) Uani 1 1 d . . . . .
U4 U 0.79268(9) 0.36053(7) 0.85674(7) 0.0131(2) Uani 1 1 d . . . . .
U5 U 0.49209(9) 0.00405(7) 0.80796(7) 0.0149(2) Uani 1 1 d . . . . .
U6 U 0.500000 0.000000 0.500000 0.0149(3) Uani 1 2 d S . P . .
Y1 Y 1.0109(3) 0.0775(2) 0.7739(2) 0.0229(4) Uani 1 1 d . . . . .
O1 O 0.3741(18) 0.7622(14) 1.0528(14) 0.0223(6) Uani 1 1 d . . . . .
O2 O 0.0420(18) 0.5582(14) 0.6275(14) 0.0223(6) Uani 1 1 d . . . . .
O3 O 0.0934(18) 0.7787(14) 0.8734(14) 0.0223(6) Uani 1 1 d . . . . .
O4 O 0.3471(18) 0.7745(14) 0.7391(14) 0.0223(6) Uani 1 1 d . . . . .
O5 O 0.3581(18) 0.5552(14) 0.8022(14) 0.0223(6) Uani 1 1 d . . . . .
O6 O 0.7026(18) 0.6572(14) 0.7622(14) 0.0223(6) Uani 1 1 d . . . . .
O7 O 0.3592(18) 0.3178(14) 0.5789(14) 0.0223(6) Uani 1 1 d . . . . .
O8 O 0.6279(18) 0.4469(14) 0.4758(14) 0.0223(6) Uani 1 1 d . . . . .
O9 O 0.9653(18) 0.2735(14) 0.5169(14) 0.0223(6) Uani 1 1 d . . . . .
O10 O 0.7444(18) 0.3870(14) 0.6728(14) 0.0223(6) Uani 1 1 d . . . . .
O11 O 0.6375(18) 0.4568(14) 0.8698(14) 0.0223(6) Uani 1 1 d . . . . .
O12 O 1.0602(18) 0.5427(14) 0.9211(14) 0.0223(6) Uani 1 1 d . . . . .
O13 O 0.5551(18) 0.1422(14) 0.6912(14) 0.0223(6) Uani 1 1 d . . . . .
O14 O 0.9351(18) 0.2610(14) 0.8335(14) 0.0223(6) Uani 1 1 d . . . . .
O15 O 0.7227(18) 0.0036(14) 0.8277(14) 0.0223(6) Uani 1 1 d . . . . .
O16 O 0.2623(18) 0.0130(14) 0.7765(14) 0.0223(6) Uani 1 1 d . . . . .
O17 O 0.462(3) 0.005(3) 0.994(3) 0.0223(6) Uani 0.5 1 d . . P . .
O18 O 0.4118(18) -0.1311(14) 0.5765(14) 0.0223(6) Uani 1 1 d . . . . .
O19 O 0.7793(18) 0.0076(14) 0.5783(14) 0.0223(6) Uani 1 1 d . . . . .
O20 O 1.1354(19) 0.1470(14) 0.6337(14) 0.0223(6) Uani 1 1 d . . . . .
O21 O 1.2958(18) 0.2826(14) 0.9036(14) 0.0223(6) Uani 1 1 d . . . . .
O22 O 0.8958(19) -0.1558(14) 0.6892(14) 0.0223(6) Uani 1 1 d . . . . .
O23 O 1.1150(18) 0.0961(14) 0.9848(14) 0.0223(6) Uani 1 1 d . . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
U3 U1 U2 64.04(3) 2_666 . ?
U3 U1 U4 172.79(3) 2_666 2_667 ?
U3 U1 U5 59.81(4) 2_666 1_565 ?
U3 U1 U5 126.55(3) 2_666 2_667 ?
U4 U1 U2 112.74(3) 2_667 . ?
U4 U1 U5 127.25(4) 2_667 1_565 ?
U4 U1 U5 60.46(3) 2_667 2_667 ?
U5 U1 U2 113.33(3) 2_667 . ?
U5 U1 U2 87.82(3) 1_565 . ?
U5 U1 U5 66.79(4) 2_667 1_565 ?
O1 U1 U2 103.0(3) . . ?
O1 U1 U3 147.8(3) . 2_666 ?
O1 U1 U4 37.7(3) . 2_667 ?
O1 U1 U5 28.4(3) . 2_667 ?
O1 U1 U5 91.9(3) . 1_565 ?
O1 U1 O12 73.1(5) . 1_455 ?
O2 U1 U2 78.4(3) . . ?
O2 U1 U3 36.8(3) . 2_666 ?
O2 U1 U4 137.5(3) . 2_667 ?
O2 U1 U5 154.9(3) . 2_667 ?
O2 U1 U5 92.7(3) . 1_565 ?
O2 U1 O1 175.2(5) . . ?
O2 U1 O4 72.9(5) . . ?
O2 U1 O12 102.1(5) . 1_455 ?
O3 U1 U2 158.0(4) . . ?
O3 U1 U3 96.5(4) . 2_666 ?
O3 U1 U4 87.8(4) . 2_667 ?
O3 U1 U5 69.0(4) . 2_667 ?
O3 U1 U5 72.8(4) . 1_565 ?
O3 U1 O1 88.2(6) . . ?
O3 U1 O2 91.9(6) . . ?
O3 U1 O4 89.6(5) . . ?
O3 U1 O5 176.5(6) . . ?
O3 U1 O12 90.3(5) . 1_455 ?
O4 U1 U2 68.7(3) . . ?
O4 U1 U3 36.8(4) . 2_666 ?
O4 U1 U4 149.6(4) . 2_667 ?
O4 U1 U5 90.4(4) . 2_667 ?
O4 U1 U5 25.5(4) . 1_565 ?
O4 U1 O1 111.9(5) . . ?
O4 U1 O12 175.0(5) . 1_455 ?
O5 U1 U2 19.9(4) . . ?
O5 U1 U3 82.7(4) . 2_666 ?
O5 U1 U4 93.4(4) . 2_667 ?
O5 U1 U5 108.8(4) . 2_667 ?
O5 U1 U5 103.9(4) . 1_565 ?
O5 U1 O1 90.7(5) . . ?
O5 U1 O2 89.4(5) . . ?
O5 U1 O4 87.7(5) . . ?
O5 U1 O12 92.5(5) . 1_455 ?
O12 U1 U2 110.9(3) 1_455 . ?
O12 U1 U3 138.3(4) 1_455 2_666 ?
O12 U1 U4 35.4(4) 1_455 2_667 ?
O12 U1 U5 158.0(4) 1_455 1_565 ?
O12 U1 U5 94.3(4) 1_455 2_667 ?
U2 U2 U1 105.93(3) 2_666 . ?
U3 U2 U1 170.43(2) . . ?
U3 U2 U2 64.73(3) . 2_666 ?
U4 U2 U1 117.47(3) . . ?
U4 U2 U2 136.59(3) . 2_666 ?
U4 U2 U3 71.87(3) . . ?
O5 U2 U1 16.3(3) . . ?
O5 U2 U2 121.2(3) . 2_666 ?
O5 U2 U3 173.1(3) . . ?
O5 U2 U4 102.1(3) . . ?
O5 U2 O8 154.6(4) . . ?
O5 U2 O8 85.9(5) . 2_666 ?
O5 U2 O11 73.7(5) . . ?
O6 U2 U1 82.9(4) . . ?
O6 U2 U2 91.0(4) . 2_666 ?
O6 U2 U3 94.9(4) . . ?
O6 U2 U4 93.5(4) . . ?
O6 U2 O5 88.7(5) . . ?
O6 U2 O7 178.8(6) . . ?
O6 U2 O8 92.1(5) . . ?
O6 U2 O8 89.5(5) . 2_666 ?
O6 U2 O10 94.7(5) . . ?
O6 U2 O11 88.0(5) . . ?
O7 U2 U1 96.9(4) . . ?
O7 U2 U2 87.9(4) . 2_666 ?
O7 U2 U3 85.2(4) . . ?
O7 U2 U4 87.6(4) . . ?
O7 U2 O5 91.4(5) . . ?
O7 U2 O8 89.4(5) . 2_666 ?
O7 U2 O8 87.3(5) . . ?
O7 U2 O10 86.0(5) . . ?
O7 U2 O11 93.2(5) . . ?
O8 U2 U1 70.8(3) 2_666 . ?
O8 U2 U1 139.2(3) . . ?
O8 U2 U2 33.5(3) . 2_666 ?
O8 U2 U2 35.3(3) 2_666 2_666 ?
O8 U2 U3 100.0(3) 2_666 . ?
O8 U2 U3 31.3(3) . . ?
O8 U2 U4 171.5(3) 2_666 . ?
O8 U2 U4 103.2(3) . . ?
O8 U2 O8 68.8(5) 2_666 . ?
O8 U2 O11 159.5(4) 2_666 . ?
O10 U2 U1 153.6(3) . . ?
O10 U2 U2 100.4(3) . 2_666 ?
O10 U2 U3 35.6(3) . . ?
O10 U2 U4 36.2(3) . . ?
O10 U2 O5 138.3(5) . . ?
O10 U2 O8 66.9(4) . . ?
O10 U2 O8 135.6(5) . 2_666 ?
O10 U2 O11 64.9(5) . . ?
O11 U2 U1 88.7(3) . . ?
O11 U2 U2 165.1(3) . 2_666 ?
O11 U2 U3 100.5(3) . . ?
O11 U2 U4 28.8(3) . . ?
O11 U2 O8 131.7(5) . . ?
U1 U3 U2 125.19(3) 2_666 . ?
U1 U3 U3 67.79(5) 2_666 2_766 ?
U1 U3 U5 65.64(4) 2_666 2_656 ?
U2 U3 U3 109.95(4) . 2_766 ?
U2 U3 U5 112.00(4) . 2_656 ?
U3 U3 U5 129.54(4) 2_766 2_656 ?
O2 U3 U1 34.4(3) 2_666 2_666 ?
O2 U3 U1 102.2(3) 1_655 2_666 ?
O2 U3 U2 128.8(3) 2_666 . ?
O2 U3 U2 86.0(3) 1_655 . ?
O2 U3 U3 34.1(3) 2_666 2_766 ?
O2 U3 U3 34.8(3) 1_655 2_766 ?
O2 U3 U5 161.8(3) 1_655 2_656 ?
O2 U3 U5 96.2(3) 2_666 2_656 ?
O2 U3 O2 69.0(6) 1_655 2_666 ?
O2 U3 O4 137.1(5) 1_655 2_666 ?
O2 U3 O18 155.6(5) 1_655 2_656 ?
O2 U3 O18 131.6(5) 2_666 2_656 ?
O4 U3 U1 34.9(3) 2_666 2_666 ?
O4 U3 U2 116.0(3) 2_666 . ?
O4 U3 U3 102.6(3) 2_666 2_766 ?
O4 U3 U5 32.6(3) 2_666 2_656 ?
O4 U3 O2 68.7(5) 2_666 2_666 ?
O4 U3 O18 66.4(5) 2_666 2_656 ?
O8 U3 U1 85.2(4) . 2_666 ?
O8 U3 U2 40.1(4) . . ?
O8 U3 U3 93.5(4) . 2_766 ?
O8 U3 U5 100.9(4) . 2_656 ?
O8 U3 O2 91.0(5) . 1_655 ?
O8 U3 O2 94.7(5) . 2_666 ?
O8 U3 O4 85.8(5) . 2_666 ?
O8 U3 O10 77.5(5) . . ?
O8 U3 O18 99.0(5) . 2_656 ?
O9 U3 U1 101.5(4) . 2_666 ?
O9 U3 U2 133.2(4) . . ?
O9 U3 U3 88.8(4) . 2_766 ?
O9 U3 U5 82.4(4) . 2_656 ?
O9 U3 O2 87.2(5) . 1_655 ?
O9 U3 O2 90.8(5) . 2_666 ?
O9 U3 O4 99.9(5) . 2_666 ?
O9 U3 O8 173.3(6) . . ?
O9 U3 O10 95.8(5) . . ?
O9 U3 O18 80.2(5) . 2_656 ?
O10 U3 U1 162.4(3) . 2_666 ?
O10 U3 U2 37.4(3) . . ?
O10 U3 U3 115.9(4) . 2_766 ?
O10 U3 U5 114.4(4) . 2_656 ?
O10 U3 O2 149.3(5) . 2_666 ?
O10 U3 O2 81.4(5) . 1_655 ?
O10 U3 O4 138.6(5) . 2_666 ?
O10 U3 O18 79.1(5) . 2_656 ?
O18 U3 U1 100.8(3) 2_656 2_666 ?
O18 U3 U2 87.4(3) 2_656 . ?
O18 U3 U3 162.5(3) 2_656 2_766 ?
O18 U3 U5 35.7(3) 2_656 2_656 ?
U1 U4 U4 70.57(4) 2_667 2_767 ?
U1 U4 U5 64.20(4) 2_667 . ?
U1 U4 Y1 89.32(4) 2_667 . ?
U2 U4 U1 129.50(3) . 2_667 ?
U2 U4 U4 112.20(4) . 2_767 ?
U2 U4 U5 112.31(4) . . ?
U2 U4 Y1 136.97(4) . . ?
U4 U4 U5 130.09(4) 2_767 . ?
U4 U4 Y1 96.50(5) 2_767 . ?
U5 U4 Y1 63.93(3) . . ?
O1 U4 U1 35.0(3) 2_667 2_667 ?
O1 U4 U2 114.2(3) 2_667 . ?
O1 U4 U4 105.5(3) 2_667 2_767 ?
O1 U4 U5 33.7(3) 2_667 . ?
O1 U4 Y1 86.1(3) 2_667 . ?
O1 U4 O13 66.6(5) 2_667 . ?
O10 U4 U1 167.6(3) . 2_667 ?
O10 U4 U2 38.3(3) . . ?
O10 U4 U4 113.9(4) . 2_767 ?
O10 U4 U5 114.8(4) . . ?
O10 U4 Y1 101.4(3) . . ?
O10 U4 O1 138.5(5) . 2_667 ?
O10 U4 O12 147.3(5) . 2_767 ?
O10 U4 O12 80.1(5) . . ?
O10 U4 O13 77.5(5) . . ?
O11 U4 U1 91.6(4) . 2_667 ?
O11 U4 U2 38.4(4) . . ?
O11 U4 U4 96.5(4) . 2_767 ?
O11 U4 U5 104.5(4) . . ?
O11 U4 Y1 166.5(4) . . ?
O11 U4 O1 86.9(5) . 2_667 ?
O11 U4 O10 76.5(5) . . ?
O11 U4 O12 93.6(5) . 2_767 ?
O11 U4 O12 97.1(5) . . ?
O11 U4 O13 96.1(5) . . ?
O12 U4 U1 105.3(3) . 2_667 ?
O12 U4 U1 35.3(3) 2_767 2_667 ?
O12 U4 U2 91.1(3) . . ?
O12 U4 U2 127.1(3) 2_767 . ?
O12 U4 U4 35.3(3) 2_767 2_767 ?
O12 U4 U4 34.8(3) . 2_767 ?
O12 U4 U5 97.8(3) 2_767 . ?
O12 U4 U5 156.0(3) . . ?
O12 U4 Y1 95.7(3) . . ?
O12 U4 Y1 94.9(3) 2_767 . ?
O12 U4 O1 140.3(5) . 2_667 ?
O12 U4 O1 70.2(5) 2_767 2_667 ?
O12 U4 O12 70.1(5) 2_767 . ?
O12 U4 O13 135.0(5) 2_767 . ?
O12 U4 O13 150.6(5) . . ?
O13 U4 U1 100.5(3) . 2_667 ?
O13 U4 U2 83.1(3) . . ?
O13 U4 U4 164.7(3) . 2_767 ?
O13 U4 U5 37.3(3) . . ?
O13 U4 Y1 70.5(3) . . ?
O14 U4 U1 90.9(4) . 2_667 ?
O14 U4 U2 138.8(4) . . ?
O14 U4 U4 86.5(4) . 2_767 ?
O14 U4 U5 74.5(4) . . ?
O14 U4 Y1 11.3(4) . . ?
O14 U4 O1 93.8(5) . 2_667 ?
O14 U4 O10 100.9(5) . . ?
O14 U4 O11 176.6(6) . . ?
O14 U4 O12 89.8(6) . 2_767 ?
O14 U4 O12 84.6(5) . . ?
O14 U4 O13 81.2(5) . . ?
U3 U5 U1 167.59(3) 2_656 2_667 ?
U3 U5 U4 136.86(4) 2_656 . ?
U4 U5 U1 55.34(3) . 2_667 ?
U6 U5 U1 123.49(3) . 2_667 ?
U6 U5 U3 68.62(3) . 2_656 ?
U6 U5 U4 68.24(4) . . ?
O1 U5 U1 26.7(3) 2_667 2_667 ?
O1 U5 U3 164.3(3) 2_667 2_656 ?
O1 U5 U4 34.2(3) 2_667 . ?
O1 U5 U6 100.5(3) 2_667 . ?
O1 U5 O13 66.4(5) 2_667 . ?
O1 U5 O18 133.8(5) 2_667 . ?
O4 U5 U1 135.0(3) 1_545 2_667 ?
O4 U5 U3 32.7(3) 1_545 2_656 ?
O4 U5 U4 165.2(3) 1_545 . ?
O4 U5 U6 99.9(3) 1_545 . ?
O4 U5 O1 159.5(4) 1_545 2_667 ?
O4 U5 O13 133.7(5) 1_545 . ?
O4 U5 O18 66.6(5) 1_545 . ?
O13 U5 U1 91.1(3) . 2_667 ?
O13 U5 U3 101.3(3) . 2_656 ?
O13 U5 U4 36.6(3) . . ?
O13 U5 U6 34.4(3) . . ?
O15 U5 U1 80.5(4) . 2_667 ?
O15 U5 U3 99.7(4) . 2_656 ?
O15 U5 U4 75.1(4) . . ?
O15 U5 U6 82.7(4) . . ?
O15 U5 O1 89.7(5) . 2_667 ?
O15 U5 O4 95.1(5) . 1_545 ?
O15 U5 O13 87.2(5) . . ?
O15 U5 O16 174.0(6) . . ?
O15 U5 O17 102.3(7) . . ?
O15 U5 O17 85.8(7) . 2_657 ?
O15 U5 O18 86.3(5) . . ?
O16 U5 U1 100.5(4) . 2_667 ?
O16 U5 U3 80.7(4) . 2_656 ?
O16 U5 U4 100.5(4) . . ?
O16 U5 U6 91.9(4) . . ?
O16 U5 O1 88.7(5) . 2_667 ?
O16 U5 O4 88.4(5) . 1_545 ?
O16 U5 O13 86.8(5) . . ?
O16 U5 O17 83.1(7) . . ?
O16 U5 O17 99.7(7) . 2_657 ?
O16 U5 O18 90.6(5) . . ?
O17 U5 U1 56.8(8) 2_657 2_667 ?
O17 U5 U1 58.4(8) . 2_667 ?
O17 U5 U3 110.8(8) 2_657 2_656 ?
O17 U5 U3 109.8(8) . 2_656 ?
O17 U5 U4 113.2(8) . . ?
O17 U5 U4 111.5(8) 2_657 . ?
O17 U5 U6 168.2(6) 2_657 . ?
O17 U5 U6 175.0(6) . . ?
O17 U5 O1 82.2(8) 2_657 2_667 ?
O17 U5 O1 80.1(8) . 2_667 ?
O17 U5 O4 79.4(9) . 1_545 ?
O17 U5 O4 78.2(8) 2_657 1_545 ?
O17 U5 O13 145.2(8) . . ?
O17 U5 O13 147.9(8) 2_657 . ?
O17 U5 O17 16.6(11) . 2_657 ?
O17 U5 O18 143.0(8) 2_657 . ?
O17 U5 O18 145.6(8) . . ?
O18 U5 U1 155.4(3) . 2_667 ?
O18 U5 U3 35.9(3) . 2_656 ?
O18 U5 U4 101.2(3) . . ?
O18 U5 U6 33.3(3) . . ?
O18 U5 O13 67.4(5) . . ?
U5 U6 U5 180.0 . 2_656 ?
O13 U6 U5 41.9(4) 2_656 2_656 ?
O13 U6 U5 41.9(4) . . ?
O13 U6 U5 138.1(4) 2_656 . ?
O13 U6 U5 138.1(4) . 2_656 ?
O13 U6 O13 180.0(11) 2_656 . ?
O13 U6 O19 86.5(5) 2_656 2_656 ?
O13 U6 O19 93.5(5) . 2_656 ?
O13 U6 O19 93.5(5) 2_656 . ?
O13 U6 O19 86.5(5) . . ?
O18 U6 U5 140.4(4) . 2_656 ?
O18 U6 U5 39.6(4) 2_656 2_656 ?
O18 U6 U5 39.6(4) . . ?
O18 U6 U5 140.4(4) 2_656 . ?
O18 U6 O13 81.1(5) . . ?
O18 U6 O13 98.9(5) 2_656 . ?
O18 U6 O13 81.1(5) 2_656 2_656 ?
O18 U6 O13 98.9(5) . 2_656 ?
O18 U6 O18 180.0 2_656 . ?
O18 U6 O19 92.3(5) 2_656 . ?
O18 U6 O19 87.7(5) . . ?
O18 U6 O19 87.7(5) 2_656 2_656 ?
O18 U6 O19 92.3(5) . 2_656 ?
O19 U6 U5 98.2(3) 2_656 . ?
O19 U6 U5 81.8(3) 2_656 2_656 ?
O19 U6 U5 81.8(3) . . ?
O19 U6 U5 98.2(3) . 2_656 ?
O19 U6 O19 180.0 . 2_656 ?
O14 Y1 U4 9.1(3) . . ?
O14 Y1 O15 74.7(4) . . ?
O14 Y1 O16 143.2(5) . 1_655 ?
O14 Y1 O19 81.3(5) . . ?
O14 Y1 O20 88.7(5) . . ?
O14 Y1 O21 72.0(5) . . ?
O14 Y1 O22 144.0(5) . . ?
O14 Y1 O23 96.0(5) . . ?
O15 Y1 U4 66.9(3) . . ?
O16 Y1 U4 152.3(3) 1_655 . ?
O16 Y1 O15 134.8(4) 1_655 . ?
O16 Y1 O21 71.5(5) 1_655 . ?
O19 Y1 U4 75.5(3) . . ?
O19 Y1 O15 77.5(5) . . ?
O19 Y1 O16 121.2(5) . 1_655 ?
O19 Y1 O20 70.5(5) . . ?
O19 Y1 O21 131.5(5) . . ?
O19 Y1 O22 77.6(5) . . ?
O19 Y1 O23 151.6(5) . . ?
O20 Y1 U4 93.2(3) . . ?
O20 Y1 O15 145.9(5) . . ?
O20 Y1 O16 74.5(5) . 1_655 ?
O20 Y1 O21 69.2(5) . . ?
O21 Y1 U4 81.0(3) . . ?
O21 Y1 O15 129.6(5) . . ?
O22 Y1 U4 134.9(3) . . ?
O22 Y1 O15 72.4(4) . . ?
O22 Y1 O16 72.7(5) . 1_655 ?
O22 Y1 O20 110.8(5) . . ?
O22 Y1 O21 142.6(5) . . ?
O22 Y1 O23 89.3(5) . . ?
O23 Y1 U4 97.8(3) . . ?
O23 Y1 O15 74.6(4) . . ?
O23 Y1 O16 77.1(5) . 1_655 ?
O23 Y1 O20 137.8(5) . . ?
O23 Y1 O21 72.6(5) . . ?
U1 O1 U4 107.3(5) . 2_667 ?
U1 O1 U5 124.9(6) . 2_667 ?
U5 O1 U4 112.1(6) 2_667 2_667 ?
U1 O2 U3 137.2(6) . 1_455 ?
U1 O2 U3 108.7(6) . 2_666 ?
U3 O2 U3 111.0(6) 1_455 2_666 ?
U1 O4 U3 108.3(6) . 2_666 ?
U1 O4 U5 130.2(6) . 1_565 ?
U5 O4 U3 114.7(5) 1_565 2_666 ?
U1 O5 U2 143.8(7) . . ?
U2 O8 U2 111.2(5) 2_666 . ?
U3 O8 U2 140.0(7) . 2_666 ?
U3 O8 U2 108.6(5) . . ?
U3 O10 U2 107.0(5) . . ?
U4 O10 U2 105.5(5) . . ?
U4 O10 U3 147.6(6) . . ?
U4 O11 U2 112.7(6) . . ?
U1 O12 U4 109.3(6) 1_655 2_767 ?
U1 O12 U4 140.7(6) 1_655 . ?
U4 O12 U4 109.9(5) 2_767 . ?
U4 O13 U5 106.1(5) . . ?
U6 O13 U4 137.8(6) . . ?
U6 O13 U5 103.7(5) . . ?
U4 O14 Y1 159.7(7) . . ?
U5 O15 Y1 145.7(6) . . ?
U5 O16 Y1 166.7(8) . 1_455 ?
U5 O17 U5 163.4(11) . 2_657 ?
O17 O17 U5 76(5) 2_657 2_657 ?
O17 O17 U5 87(5) 2_657 . ?
U5 O18 U3 108.4(5) . 2_656 ?
U6 O18 U3 141.9(7) . 2_656 ?
U6 O18 U5 107.0(6) . . ?
U6 O19 Y1 141.6(7) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 U2 4.0871(14) . ?
U1 U3 3.6255(11) 2_666 ?
U1 U4 3.6516(11) 2_667 ?
U1 U5 4.0542(15) 1_565 ?
U1 U5 3.997(3) 2_667 ?
U1 O1 2.192(14) . ?
U1 O2 2.165(14) . ?
U1 O3 1.821(13) . ?
U1 O4 2.186(13) . ?
U1 O5 1.939(13) . ?
U1 O12 2.234(13) 1_455 ?
U2 U2 4.0040(15) 2_666 ?
U2 U3 3.6501(13) . ?
U2 U4 3.6035(13) . ?
U2 O5 2.358(13) . ?
U2 O6 1.760(14) . ?
U2 O7 1.785(14) . ?
U2 O8 2.369(13) 2_666 ?
U2 O8 2.481(13) . ?
U2 O10 2.318(13) . ?
U2 O11 2.429(13) . ?
U3 U3 3.751(2) 2_766 ?
U3 U5 3.847(3) 2_656 ?
U3 O2 2.255(14) 1_655 ?
U3 O2 2.295(13) 2_666 ?
U3 O4 2.285(14) 2_666 ?
U3 O8 2.001(13) . ?
U3 O9 1.843(13) . ?
U3 O10 2.224(13) . ?
U3 O18 2.378(13) 2_656 ?
U4 U4 3.699(3) 2_767 ?
U4 U5 3.8626(18) . ?
U4 Y1 4.026(2) . ?
U4 O1 2.341(13) 2_667 ?
U4 O10 2.210(13) . ?
U4 O11 1.884(13) . ?
U4 O12 2.244(14) 2_767 ?
U4 O12 2.275(13) . ?
U4 O13 2.399(14) . ?
U4 O14 1.830(14) . ?
U5 U6 3.5457(10) . ?
U5 O1 2.315(14) 2_667 ?
U5 O4 2.283(13) 1_545 ?
U5 O13 2.436(13) . ?
U5 O15 1.829(13) . ?
U5 O16 1.851(13) . ?
U5 O17 2.21(3) . ?
U5 O17 2.27(3) 2_657 ?
U5 O18 2.366(14) . ?
U6 O13 2.063(14) 2_656 ?
U6 O13 2.063(14) . ?
U6 O18 2.038(13) . ?
U6 O18 2.038(13) 2_656 ?
U6 O19 2.200(13) . ?
U6 O19 2.200(13) 2_656 ?
Y1 O14 2.260(14) . ?
Y1 O15 2.539(13) . ?
Y1 O16 2.348(13) 1_655 ?
Y1 O19 2.277(14) . ?
Y1 O20 2.336(14) . ?
Y1 O21 2.429(14) . ?
Y1 O22 2.285(13) . ?
Y1 O23 2.293(13) . ?
O17 O17 0.65(4) 2_657 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
U1 U4 O11 U2 -171.5(5) 2_667 . . . ?
U1 U4 O14 Y1 82(2) 2_667 . . . ?
U1 U5 O15 Y1 -94.8(12) 2_667 . . . ?
U1 U5 O16 Y1 19(3) 2_667 . . 1_455 ?
U2 U4 O14 Y1 -87(2) . . . . ?
U3 U5 O15 Y1 97.8(12) 2_656 . . . ?
U3 U5 O16 Y1 -174(3) 2_656 . . 1_455 ?
U4 U4 O11 U2 117.9(5) 2_767 . . . ?
U4 U4 O14 Y1 153(2) 2_767 . . . ?
U4 U5 O15 Y1 -38.3(11) . . . . ?
U4 U5 O16 Y1 -37(3) . . . 1_455 ?
U5 U4 O11 U2 -107.8(5) . . . . ?
U5 U4 O14 Y1 19(2) . . . . ?
U6 U5 O15 Y1 31.0(11) . . . . ?
U6 U5 O16 Y1 -106(3) . . . 1_455 ?
Y1 U4 O11 U2 -77.8(18) . . . . ?
O1 U4 O11 U2 -136.8(6) 2_667 . . . ?
O1 U4 O14 Y1 47(2) 2_667 . . . ?
O1 U5 O15 Y1 -69.6(12) 2_667 . . . ?
O1 U5 O16 Y1 -5(3) 2_667 . . 1_455 ?
O4 U5 O15 Y1 130.4(12) 1_545 . . . ?
O4 U5 O16 Y1 155(3) 1_545 . . 1_455 ?
O10 U4 O11 U2 4.8(5) . . . . ?
O10 U4 O14 Y1 -94(2) . . . . ?
O12 U4 O11 U2 153.3(6) 2_767 . . . ?
O12 U4 O11 U2 82.9(6) . . . . ?
O12 U4 O14 Y1 117(2) 2_767 . . . ?
O12 U4 O14 Y1 -173(2) . . . . ?
O13 U4 O11 U2 -70.8(6) . . . . ?
O13 U4 O14 Y1 -18(2) . . . . ?
O13 U5 O15 Y1 -3.2(12) . . . . ?
O13 U5 O16 Y1 -71(3) . . . 1_455 ?
O17 U5 O15 Y1 -149.4(14) . . . . ?
O17 U5 O15 Y1 -151.8(14) 2_657 . . . ?
O17 U5 O16 Y1 75(3) . . . 1_455 ?
O17 U5 O16 Y1 77(3) 2_657 . . 1_455 ?
O18 U5 O15 Y1 64.3(12) . . . . ?
O18 U5 O16 Y1 -139(3) . . . 1_455 ?
